General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.77 - 7.9 g/cm³ Show Material materials with Density of 7.77 - 7.9 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa |

20.0 °C | 196 GPa Show Material materials with Elastic modulus of 196 GPa | |

24.0 °C | 193.7 GPa Show Material materials with Elastic modulus of 193.7 GPa | |

100.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | |

200.0 °C | 182 GPa Show Material materials with Elastic modulus of 182 GPa | |

300.0 °C | 174 GPa Show Material materials with Elastic modulus of 174 GPa | |

400.0 °C | 166 GPa Show Material materials with Elastic modulus of 166 GPa | |

500.0 °C | 158 GPa Show Material materials with Elastic modulus of 158 GPa | |

600.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

700.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | |

800.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | |

900.0 °C | 127 GPa Show Material materials with Elastic modulus of 127 GPa | |

1000.0 °C | 120 GPa Show Material materials with Elastic modulus of 120 GPa | |

Elongation | 20.0 °C | 35 % Show Material materials with Elongation of 35 % |

Elongation A80 | 20.0 °C | 33 % Show Material materials with Elongation A80 of 33 % |

Hardness, Brinell | 20.0 °C | 192 [-] Show Material materials with Hardness, Brinell of 192 [-] |

Poisson's ratio | 24.0 °C | 0.23 - 0.24 [-] Show Material materials with Poisson's ratio of 0.23 - 0.24 [-] |

Shear modulus | 24.0 °C | 74.5 - 77.9 GPa Show Material materials with Shear modulus of 74.5 - 77.9 GPa |

Tensile strength | 20.0 °C | 500 - 700 MPa Show Material materials with Tensile strength of 500 - 700 MPa |

Yield strength Rp0.2 | 20.0 °C | 210 MPa Show Material materials with Yield strength Rp0.2 of 210 MPa |

Yield strength Rp1.0 | 20.0 °C | 250 MPa Show Material materials with Yield strength Rp1.0 of 250 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.67E-5 1/K | ||

200.0 °C | 1.6E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.77E-5 1/K | ||

400.0 °C | 1.75E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.75E-5 - 1.81E-5 1/K | ||

500.0 °C | 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.84E-5 1/K | ||

600.0 °C | 1.8E-5 - 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.8E-5 - 1.88E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

800.0 °C | 1.85E-5 - 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.85E-5 - 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 1.95E-5 - 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.95E-5 - 2E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 1000 °C Show Material materials with Max service temperature, long of 0 - 1000 °C | ||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 472 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 472 - 500 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 12.6 - 15 W/(m·K) Show Material materials with Thermal conductivity of 12.6 - 15 W/(m·K) | |

100.0 °C | 14.1 W/(m·K) Show Material materials with Thermal conductivity of 14.1 W/(m·K) | ||

200.0 °C | 15.9 W/(m·K) Show Material materials with Thermal conductivity of 15.9 W/(m·K) | ||

300.0 °C | 17.4 W/(m·K) Show Material materials with Thermal conductivity of 17.4 W/(m·K) | ||

400.0 °C | 19 W/(m·K) Show Material materials with Thermal conductivity of 19 W/(m·K) | ||

500.0 °C | 19 - 20.5 W/(m·K) Show Material materials with Thermal conductivity of 19 - 20.5 W/(m·K) | ||

600.0 °C | 21.9 W/(m·K) Show Material materials with Thermal conductivity of 21.9 W/(m·K) | ||

700.0 °C | 23.3 W/(m·K) Show Material materials with Thermal conductivity of 23.3 W/(m·K) | ||

800.0 °C | 24.7 W/(m·K) Show Material materials with Thermal conductivity of 24.7 W/(m·K) | ||

900.0 °C | 26.1 W/(m·K) Show Material materials with Thermal conductivity of 26.1 W/(m·K) | ||

1000.0 °C | 27.5 W/(m·K) Show Material materials with Thermal conductivity of 27.5 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.4 mm²/s Show Material materials with Thermal diffusivity of 3.4 mm²/s | |

100.0 °C | 3.6 mm²/s Show Material materials with Thermal diffusivity of 3.6 mm²/s | ||

200.0 °C | 3.9 mm²/s Show Material materials with Thermal diffusivity of 3.9 mm²/s | ||

300.0 °C | 4.3 mm²/s Show Material materials with Thermal diffusivity of 4.3 mm²/s | ||

400.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

500.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

600.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

700.0 °C | 5.1 mm²/s Show Material materials with Thermal diffusivity of 5.1 mm²/s | ||

800.0 °C | 5.5 mm²/s Show Material materials with Thermal diffusivity of 5.5 mm²/s | ||

900.0 °C | 5.8 mm²/s Show Material materials with Thermal diffusivity of 5.8 mm²/s | ||

1000.0 °C | 5.9 mm²/s Show Material materials with Thermal diffusivity of 5.9 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.8E-7 - 8.68E-7 Ω·m Show Material materials with Electrical resistivity of 7.8E-7 - 8.68E-7 Ω·m |

100.0 °C | 9.21E-7 Ω·m Show Material materials with Electrical resistivity of 9.21E-7 Ω·m | |

200.0 °C | 9.75E-7 Ω·m Show Material materials with Electrical resistivity of 9.75E-7 Ω·m | |

300.0 °C | 1.03E-6 Ω·m Show Material materials with Electrical resistivity of 1.03E-6 Ω·m | |

400.0 °C | 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 Ω·m | |

500.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

600.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

700.0 °C | 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.18E-6 Ω·m | |

800.0 °C | 1.21E-6 Ω·m Show Material materials with Electrical resistivity of 1.21E-6 Ω·m | |

900.0 °C | 1.24E-6 Ω·m Show Material materials with Electrical resistivity of 1.24E-6 Ω·m | |

1000.0 °C | 1.26E-6 Ω·m Show Material materials with Electrical resistivity of 1.26E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.15 % Show Material materials with Carbon of 0.15 % |

Chromium | 22 - 24 % Show Material materials with Chromium of 22 - 24 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Nickel | 12 - 14 % Show Material materials with Nickel of 12 - 14 % |

Nitrogen | 0.11 % Show Material materials with Nitrogen of 0.11 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |